1 40 The Open Orthopaedics Journal, 2009, 3, Open Access An Ultrasound Assisted Anchoring Technique (BoneWelding Technology) for Fixation of Implants to Bone A Histological Pilot Study in Sheep Jens D. Langhoff *,1,2, Jan M. Kuemmerle 1, Joerg Mayer 2, Urs Weber 2, Milica Berra 2, Jessika M. Mueller 3, Sabine B. Kaestner 4, Katalin Zlinszky 1, Joerg A. Auer 1, Brigitte von Rechenberg 1 1 Musculoskeletal Research Unit, Equine Hospital, Vetsuisse Faculty ZH, University of Zurich, Winterthurerstr. 260, CH-8057 Zurich, Switzerland 2 WW Technology AG, Wagistr. 6, CH-8952 Schlieren, Switzerland 3 University of Veterinary Medicine Hannover, Horse Clinic, Bischofsholer Damm 15, Hannover, Germany 4 University of Vseterinary Medicine Hannover, Small Animal Clinic, Bischofsholer Damm 15, Hannover, Germany Abstract: The BoneWelding Technology offers new opportunities to anchor implants within bone. The technology melted the surface of biodegradable polymer pins by means of ultrasound energy to mould material into the structures of the predrilled bone. Temperature changes were measured at the sites of implantation in an in vitro experiment. In the in vivo part of the study two types of implants were implanted in the limb of sheep to investigate the biocompatibility of the method. One implant type was made of PL-DL-lactide (PLA), the second one was a titanium core partially covered with PLA. Healing period was 2 and 6 months, with 3 sheep per group. Bone samples were evaluated radiologically, histologically and histomorphometrically for bone remodeling and inflammatory reactions. Results demonstrated mild and short temperature increase during insertion. New bone formed at the implant without evidence of inflammatory reaction. The amount of adjacent bone was increased compared to normal cancellous bone. It was concluded that the BoneWelding Technology proved to be a biocompatible technology to anchor biodegradable as well as titanium-pla implants in bone. Keywords: Implants, ultrasound, polylactide, histology, in vivo. INTRODUCTION The anchorage of implants in bone is an integral part of modern fixation techniques in orthopedics. Metal implants usually fulfill all requirements in healthy and normal bone. However, if bone structure is weak, the holding power may not be sufficient for a stable fixation [1, 2]. In osteoporotic bone mechanical stability is a great challenge with a decrease in bone mass and increased brittleness . Methods for immediate and overall improved primary stability are required to meet these challenges emerging with an increasingly aging population. The ultrasound assisted anchoring technology (BoneWelding technology) has been developed to address this problem. It combines the liquefaction and resorbability of a polymer to achieve better stability compared to screws alone. The ultrasonic vibrations cause liquefaction of the polymer in contact with the bone (Fig. 1). The liquid phase infiltrates the cancellous cavities of the adjacent bone and adheres to the structures. Re-solidification initiates as soon as the supply of ultrasonic energy is stopped. *Address correspondence to this author at the Musculoskeletal Research Unit, Equine Hospital, Vetsuisse Faculty ZH, University of Zurich, Winterthurerstr. 260, 8057 Zurich, Switzerland; Tel: ; Fax: ; s: Biomechanical tests in healthy and osteoporotic human cadaver and synthetic bones already demonstrated improved mechanical anchorage of the polymeric implants that were inserted using the BoneWelding technique compared to conventional metal screws [4, 5]. This study included an in vitro part for temperature measurements on cadaver bone and an in vivo part in sheep to evaluate the biocompatibility of the technology after medium term implantation periods. The in vitro insertions were undertaken to quantify the thermal impact and compare it to heat exposure during drilling [6, 7]. The same setup was used in the in vivo part to test for signs of potential damage to the adjacent bone due to heat generated by insertion. The primary focus of the present study was the in vivobiocompatibility of the ultrasonic insertion by means of qualitative histological assessment of bone response. It was assumed that the excellent biocompatibility of the implant components, PLA [8, 9] and titanium [10, 11], would not be altered by the insertion technique. Possible changes in tissue reaction could then be attributed to the ultrasound induced liquefaction process alone. A poly-l-dl-lactide was used as polymeric cylindrical dowel implant in both parts and in the in vivo part also a partial PLA coated titanium implant (Ti-PLA) was investigated. The Ti-PLA pin had a similar, dowel like form as the polymer pin and the coating was of the same PLA material. The diameter was smaller, which lead to a gap between the drilled bone cavity and the / Bentham Open
2 BoneWelding Technology for Fixation of Implants to Bone The Open Orthopaedics Journal, 2009, Volume 3 41 Fig. (1). An active ultrasonic sonotrode drives the polymer pin into the bone (a). Heat generating shearing forces at the contact face (b) liquefy polymer, which penetrates into the bone spaces (c, d). titanium surface. This design facilitated anchoring only by the polymer part and avoided direct transmission of ultrasonic energy from metal to bone as an unknown factor in the setup. The performance of implants was tested in cancellous and cortical bone to establish results for several clinical applications. MATERIALS AND METHODOLOGY Implants The PLA pin consisted of a co-polymer of 70% L-lactide and 30% DL-lactide (Poly-L-DL-Lactide, Resomer LR 708, Boehringer Ingelheim, Germany) which was molded into a cylindrical dowel of 3.5 mm diameter with a tapered tip and 25 mm length (Fig. 2). The titanium-pla implants had a length of 10 mm and a diameter of 2.8 mm. The implant was machined out of grade 4 titanium and surface treated by gridblasting and subsequent acid etching. Polymer was layered at the surface in small stripes (1 mm in width, 5 mm in length, and 1 mm in height) at 180 opposite of each other through a thermal sintering process. The remaining 5-mm titanium surface of the Ti-PLA implant was left uncovered. At the proximal end a thread was introduced at the inside, where an adapter piece could be introduced to serve as a coupling device to the sonotrode tip of the ultrasound equipment. After insertion and removal of the ultrasound device the adapter was replaced by a small screw. The diameter of the implants was calculated such, that enough material was available to infiltrate the surrounding bone. The implants were sterilized using gamma irradiation ( 60 Co-radiation, 25kGy). Ultrasound Device A commercially available ultrasound device was used (Branson E-150, Branson Ultrasonics SA, Carouge, Switzerland; 20kHz, amplitude of max. 60 m = 150W, set at 50%). The device was covered with a sterile plastic cover (rolled arthroscopy camera drape, mtp GmbH, Tuttlingen, Germany). The metallic implant holder of the device was disinfected using alcohol and chlorhexidine (Hibiscrub, SSL Healthcare, Switzerland). Fig. (2). Pictures of the implants. The pure PLA-pin (top) was fixed directly at the sonotrode, while an adaptor was used for the titanium-pla pin (Ti-PLA)(bottom, above the millimeter scale). Polymer stripes were sintered at the titanium core. In Vitro Temperature Measurements An in vitro study was conducted to document the thermal conditions of implantation in the osseous tissue close to the implant-bone interface. The same setup was used as in the in vivo part, but with fresh thawed sheep tibiae and femora. Bones where kept at 37 C, clamped fully submerged in a water basin. In total 3 femora and 4 tibiae were investigated, leading to 7 to 8 insertions for each area. Four equally spaced 0.5 mm holes were drilled parallel to the implantation hole at a distance of 3 mm from center point to center point. The distance between the initial pin surface and thermocouple (Sheathed thermocouple, J Type, ø 0.5 mm, MDW, Switzerland) was therefore about 1 mm. The depth of the thermocouple holes was 3 mm. Reference temperature was measured in a distance of 2 cm from the pin hole. Data were collected 17 to 18 times per second (Agilent 34970A Data Acquisition Switch Unit, Santa Clara, CA, USA) for
3 42 The Open Orthopaedics Journal, 2009, Volume 3 Langhoff et al. app. 60 seconds, starting 10 seconds before insertion. Measurements were visualized by box plots. Animal Model Six adult, female Swiss Alpine sheep between 2-4 years of age and with an average weight of 71 kg (range kg) served as well established animal model for human bone healing [12-15]. Animal experiment was conducted according to the Swiss Law of animal protection and welfare and was permitted through the official, Swiss authorities (permission # 92/2002). Perioperative care, inhalation anesthesia and postoperative analgesia and antibiosis was performed according to standard protocols as described elsewhere . Animals were sacrificed after 2 and 6 months period with 3 animals per time point. A total of 48 implants were placed in the distal femur and proximal tibia. The target areas (Fig. 3) were chosen such that 8 implants per sheep, 4 of each type, were placed in cancellous and cortical bone to test in various bone types. Each area contained one PLA and one Ti-PLA implant. Minimum distance between all implants was 10 mm. Implant cavities were prepared by drilling (3 mm in diameter, 10 mm depth) and additional tapping in cortical areas (tap for 3.5 mm cortex screws, Synthes, Oberdorf, Switzerland) to create open space for the liquefied polymer. All implants were inserted to a depth of 10 mm while applying ultrasonic energy for about 1 sec. Thereafter, the implant was left to allow re-solidification for about 10 seconds, before the tip of the sonotrode was disconnected. The protruding part of the PLA pin was cut off with a wire cutter as close to the bone surface as possible. The screw cap of the Ti-PLA implant was inserted using a special screwdriver. described elsewhere . The proximal portion of the implant including the cortex was cut lengthwise, whereas the distal portion including the cancellous bone or bone marrow was cut transversely to the implant axis exposing the full diameter of the implant. One ground section (150 m) and two thin sections (6 m) were surface stained with toluidine blue and von Kossa / McNeal method. Contact microradiographs were taken from the ground sections. Thin sections of the Ti-PLA implants were prepared as statuary example of 12 samples (6 samples per observation period). Qualitative evaluation of the histological sections was carried out microscopically (DMR, Leica, Switzerland) placing emphasis on bone resorption, new bone and fibrous tissue formation close to the implant. In addition the interface between the implant and bone was assessed carefully. Cellular aspects were analyzed in thin sections, bone morphology in ground sections. Quantitative evaluation was performed to compare changes in new bone formation adjacent to the implant observed in the qualitative evaluation in cancellous bone samples. Digital images (macroscope M 420 and digital camera DC 200, Leica, Switzerland) of ground sections that were cut longitudinally to the axis of the implant served as data source. The bone area surrounding the implant was divided in three similar sized and predefined sectors (Fig. 4) to calculate changes of bone at the implant in comparison to the bone in the periphery. Sector 1 was adjacent to the implant, sector 2 in the middle and sector three was in the periphery of the section. The extent of sector 1 was defined to cover the remodeling and new bone formation at the implant, whereas sector 2 and 3 were not influenced by remodeling and served as reference. The cancellous bone structures in the sectors were identified and colored manually (Adobe Photoshop 7.0, Adobe Systems, San Jose, CA) and all other structures were covered with a black mask to reduce false detection in image analysis software (Qwin v.1, Leica Microsystems, Cambridge, UK). Bone matrix of each side of the implant was measured separately. Bone area was calculated from the measured bone area in relation to the total area of the corresponding sector. Fig. (3). Schematic drawing of the implantation sites (1-8) in cancellous bone of the femur (area 1) and cancellous and cortical bone in the proximal tibia (area 2-4). One implant of PLA and Ti- PLA type was inserted in each area. Macroscopic and Radiographic Evaluation After sacrifice the implant sites were examined for signs of inflammation. Radiographic follow-up was performed immediately after surgery and after sacrifice of the animals. Contact radiographs (Faxitron X-Rays systems, Hewlett Packard, Oregon, USA; set at 45 kv, 1 sec) were taken in two levels of the complete bones and the singled implantation areas. Each pair of implants was cut out in blocks and processed for undecalcified bone histology as Fig. (4). Histomorphometrical bone area measurement. Bone matrix (a) was split into 3 sectors (b), sector 1 was directly at the implant. The percentage of bone in each sector was calculated with the bone area (b) and the total area (c).
4 BoneWelding Technology for Fixation of Implants to Bone The Open Orthopaedics Journal, 2009, Volume 3 43 Statistical analysis was performed to compare bone area between sectors and determine relevance of implant type, observation period and implantation areas. Analysis was performed using STATA (version 10.0, Statacorp, Texas, USA), using a general linear mode and mixed-effects restricted maximum likelihood (REML) regression. P-values <0.05 were considered to be statistically significant. Semi-quantitative evaluation was done in thin sections. Full sections were scanned for presence of osteoclasts, giant foreign body cells and lymphocytes. Cellular events were counted in regard to a reaction to the implant. RESULTS In Vitro Temperature Measurements The time dependency was characterized by a rather sharp initial peak for 10 seconds that drops back to ambient temperature in 50 to 60 seconds (Fig. 5). Small temperature differences among the thermocouples could be recorded. Maximal temperature increases between 4 to 11 C were measured with medians between 6 to 7 C. Animal Model All surgeries went well without serious complications. Implants were correctly placed at the first attempt and were seated firmly within the drill hole. Two Ti-PLA implants slipped into the bone marrow as the screw cap was tightened. They were replaced with new implants in a new drill hole. The ultrasonic equipment was user friendly, although its size was too large compared to the small implants. The time of insertion was kept as short as possible to avoid heat damage to the tissue. In the cortical bone, small portions of the liquefied polymer pushed back to the cortical surface forming a small cap around the implant. Animals recovered quickly and showed normal behavior. Macroscopic and Radiographic Evaluation All implants were firmly seated within the bone. Signs of inflammation were never noticed. Postoperative radiographs demonstrated correct placement of the implants. Radiographs after sacrifice showed implants still in place in 2 and 6 months group. At 2 months a radiodense seam with an average of 0.5 mm was clearly visible in the cancellous bone that was even more pronounced at 6 months. In cortical bone a mixture of slightly decreased and increased radiodensity was observed around the implants. Only one PLA implant (cancellous bone site at 6 months) showed a noticeable less radiodense zone. Histology The areas of radio dense material corresponded exactly with bone substance stained with toluidine blue, thus confirmed calcification of the newly formed bone. The melted polymer was pressed into the cavities of the cancellous bone, or into the threads of the cortical bone, while implants remained intact. Signs of polymer degradation could rarely be seen at 6 months. Immediate contact between implant and bone matrix was recorded without an interface membrane. New bone formation directly attached to the implant surface and ongoing remodeling was found in all histology sections, which was limited to a distance of 1 mm around the implant. Differences were found in the ratio of bone formation and remodeling between cortical and cancellous bone. In the cancellous bone area new bone formation dominated, which formed a small seam at two months that increased to a uniform bone lamella at 6 months. In cortical areas bone remodeling was more prominent as could be seen in histology sections as small, regularly distributed bone remodeling cavities within the cortex (Figs. 6, 7). The PLA pin, which was noticed in the macroradiographic evaluation, showed bone resorption and infiltration with fibrous tissue at the proximal part of the implant directly underneath the periosteum. Data of histomorphometrical evaluation were supporting the qualitative observation of remodeling in cancellous bone. Fig. (5). Typical temperature record (a) showing the short temperature peak at four thermocouples around the pin (T1-4) and the reference measurement 2 cm from the insertion point (TRef). Results of the measurements are displayed as box blot diagram of the maximal temperature differences (b) for each area in the femur (area 1) and tibia (area 2-4).
5 44 The Open Orthopaedics Journal, 2009, Volume 3 Langhoff et al. Fig. (6). Implants at 6 months in both bone qualities. In cancellous bone, the lamella of new bone at the implant was clearly visible. In cortical bone, widened osteons (arrows) indicated remodeling along the PLA implant (*) or titanium implant with polylactide stripes (*). Toluidine blue stained ground sections. Fig. (7). Representative images of new bone formation and remodeling at the PLA implant (*) after 2 months healing period; transverse section. Old bone (O) was partially resorbed and replaced by new bone formation (n, dark stained) by active remodeling units (arrows). Toluidine blue stained ground sections. Values of the sample with proximal bone resorption were in the range of the double standard deviation, and were considered as outliers and excluded from statistical analysis. For all implant types and observation periods, the bone area near the implant (Sector 1) was higher compared to the more peripheral reference sectors (2 and 3) (Fig. 8). No statistically significant differences of bone formation (measured as area) around the implants were obtained if implant types and observation periods were compared. A tendency was noticed for the inner sector (p = 0.109) and the Ti-PLA implants to show higher values (p = 0.148).
6 BoneWelding Technology for Fixation of Implants to Bone The Open Orthopaedics Journal, 2009, Volume 3 45 Fig. (8). Bone content measurements (total area/bone area) show higher values in the remodeling zone (sector 1) than in the reference zone (sectors 2 & 3). More bone was build up at Titanium-PLA compared to pure PLA pins. The cellular reaction toward both implant types was identical. At 2 and 6 months, cellular reactions attributed to inflammation were never recorded in both, cortical and cancellous bone. Active osteoblasts lined up as palisades along the newly deposited bone matrix (Fig. 9). Osteoclasts were only found located at the periosteal callus. Their number decreased over time ( 8 cells per section at 2 months, 5 cells per section at 6 months). Few foreign body cells were located directly at the implant ( 8 cells per section). Macrophages, lymphoid or plasma cells were rarely seen in the soft tissue adjacent to the bone. Typical signs of active bone remodeling including widening of the Havers system were noticed. Bone resorption zone of the single PLA implant sample was filled with loose fibrous tissue, not forming a capsule. Osteoclasts and/or osteoblasts were not present. This indicated that an ongoing process could not be found. DISCUSSION In this study it was demonstrated that the BoneWelding technology was suitable to insert implants consisting of thermoplastic polymer (PLA) into bone. The temperature increase during application of the ultrasound energy and melting of the implant surface did not cause an inflammatory reaction or hamper bone remodeling. Furthermore, this technology could be also successfully used on titanium-pla implants with excellent bone healing results. Results of the in vitro temperature measurements demonstrated a transient temperature increase of 6-7 C. This observation indicates a generally lower thermal dose compared to routine drilling procedures in bone [6, 7]. Regarding the good results of histology, the effect of the temperature increase during insertion was below the 45 C threshold for bone tissue injury [16-18] or small enough to be compensated by the repair potential of bone . Therefore, possible damage to the adjacent bone and soft tissue was considered to be negligible for the implantation success. Overall, the animal model served well for testing of implant biocompatibility, tissue damage due to generation of heat during ultrasound application in cancellous and cortical bone. The handling of the ultrasonic equipment was easy, even though the ultrasonic device used in this study was relatively large in size in relation to the small implants. Fig. (9). Remodeling unit at the polymer surface (*): Active osteoblasts (indicated by arrows) are lining newly formed calcified bone (1) (crack artifacts by microtome cutting) with a seam of osteoid in between. A single osteoclast was recorded (2). Thin section at 2 months, von Kossa/McNeal staining. The convincing performance of both implant types could be shown by all results. None of the implants broke, none of the PLA coatings sheared off. PLA melted nicely and penetrated into the bone structures. Absence of signs for polymer degradation were matching with the expected degradation behavior of the PLA, which begins with 6 months [9, 20]. The melting cap at the proximal end of the PLA pin was present throughout all cortical areas. Liquefaction of too much material may have played a role. If less porosity was present as in cortical bone, less material may have intruded into the empty bone spaces and more superfluous material may have accumulated at the cortex. If
7 46 The Open Orthopaedics Journal, 2009, Volume 3 Langhoff et al. the implant was not perfectly aligned with the drill hole, more material was stripped off and left behind during subsequent insertion. For those areas, exposition of the tissue to the implantation process was comparably high. The melting cap was also effectively shielding the underlying bone from nutrition via the periosteum. But even with this worst case scenario in cortical bone, the results were still very good. In any case, this zone never jeopardized the continuity or quality of bone nor did the cap material negatively influence the insertion quality of the technology. However, an excessive amount of material should be avoided for future application. Microscopic evaluation of the stained sections revealed excellent biocompatibility of the implants as could be expected considering the type of materials used. New bone formation with direct contact to the implant could always be assessed. Remodeling around the implants was seen in both types of implants. The area close to the implant was filled with more bone compared to non influenced bone in the periphery, indicating an early adaptation of bone morphology. The bone mass increased visibly in thickness and maturity from 2 to 6 months. Histomorphometry did not confirm these changes. This can be attributed to deviations of the trabecular bone bed or the relatively small sample size in large animal studies. Besides these common constrictions, remodeling and maturation of bone can lead to less bone over time, when initially build up woven bone was replaced by less amount of lamellar bone with higher mechanical strength. Remodeling activity of cortical bone was not exceeding normal bone healing and was comparable to those observed after normal drilling procedures [21, 22]. Titanium-PLA implants performed better compared to PLA pins. This was not surprising, since osteoblasts are known to attach and proliferate on titanium surfaces [23, 24], which may have resulted in faster deposition of new bone close to the metal part of the implant. Results of the cellular evaluation were in accordance with normal physiologic responses of bone to surgical trauma. Inflammatory cells were not visible and no fibrous interface tissue was grown between implant and bone. The few multinuclear foreign body cells at the polymer surface were not considered as an inflammatory reaction, since no other mononuclear inflammatory cells were present in the environment [25-27]. The single case of bone resorption at the proximal PLA pin was an exception, which cannot be clearly explained or attributed to the insertion method. Since no early stages of soft tissue ingrowth and bone resorption were found in any other sample, further studies need to be carefully evaluated for similar characteristics at early time points. In conclusion, the BoneWelding technology proved to be a novel, highly innovative and suitable technology for insertion of implants and repair techniques in orthopedic and trauma surgery. Future studies will have to focus on the biomechanical aspects of implant osseointegration and polymer degradation. Specific implant types and locations in the body system as well as combinations with other types of materials for bone repair will be developed. ACKNOWLEDGEMENTS The Study was funded by KTI, the Swiss Commission for Technology and Innovation. Materials were provided by the WW Technology AG, Schlieren, Switzerland. We kindly acknowledge Mr. Urs Mueller, Department of Veterinary Anatomy and Mr. Bruno Gerzner, slaughterhouse of the Vetsuisse Faculty of the University of Zurich, for their help with slaughtering and sample taking. REFERENCES  Becker W, Hujoel PP, Becker BE, Willingham H. Osteoporosis and implant failure: an exploratory case-control study. J Periodontol 2000; 71(4):  Kim WY, Han CH, Park JI, Kim JY. Failure of intertrochanteric fracture fixation with a dynamic hip screw in relation to preoperative fracture stability and osteoporosis. Int Orthop 2001; 25(6):  Lanyon L, Skerry T. Postmenopausal osteoporosis as a failure of bone's adaptation to functional loading: a hypothesis. J Bone Miner Res 2001; 16(11):  Ferguson SJ, Weber U, von Rechenberg B, Mayer J. Enhancing the mechanical integrity of the implant-bone interface with BoneWelding technology: determination of quasi-static interfacial strength and fatigue resistance. J Biomed Mater Res B Appl Biomater 2006; 77(1):  Meyer DC, Mayer J, Weber U, Mueller A, Koch PP, Gerber C. Ultrasonically implanted PLA suture anchors are stable in osteopenic bone. Clin Orthop Relat Res 2006; 442:  Eriksson AR, Albrektsson T, Albrektsson B. Heat caused by drilling cortical bone: temperature measured in vivo in patients and animals. Acta Orthop Scand 1984; 55(6):  Kondo S, Okada Y, Iseki H, et al. Thermological study of drilling bone tissue with a high-speed drill. Neurosurgery 2000; 46(5):  Heidemann W, Jeschkeit S, Ruffieux K, et al. Degradation of poly(d,l)lactide implants with or without addition of calciumphosphates in vivo. Biomaterials 2001; 22(17):  Suuronen R, Pohjonen T, Hietanen J, Lindqvist C. A 5-year in vitro and in vivo study of the biodegradation of polylactide plates. J Oral Maxillofac Surg 1998; 56(5): , discussion  Han C-H, Johansson CB, Wennerberg A, Albrektsson T. Quantitative and qualitative investigations of surface enlarged titanium and titanium alloy implants. Clin Oral Implants Res 1998; 9(1):  Buser D, Schenk RK, Steinemann S, Fiorellini JP, Fox CH, Stich H. Influence of surface characteristics on bone integration of titanium implants: a histomorphometric study in miniature pigs. J Biomed Mater Res 1991; 25(7):  Sturmer KM, Schuchardt W. New aspects of closed intramedullary nailing and marrow cavity reaming in animal experiments I: the tibia of the sheep, as a model for intramedullar nailing (author's transl). Unfallheilkunde 1980; 83(7):  Theiss F, Apelt D, Brand B, et al. Biocompatibility and resorption of a brushite calcium phosphate cement. Biomaterials 2005; 26(21):  Nunamaker DM. Experimental models of fracture repair. Clin Orthop Relat Res 1998; (355 Suppl): S  Willie BM, Bloebaum RD, Bireley WR, Bachus KN, Hofmann AA. Determining relevance of a weight-bearing ovine model for bone ingrowth assessment. J Biomed Mater Res Part A 2004; 69A(3):  Eriksson AR, Albrektsson T. Temperature threshold levels for heatinduced bone tissue injury: a vital-microscopic study in the rabbit. J Prosthet Dent 1983; 50(1):  Li S, Chien S, Branemark PI. Heat shock-induced necrosis and apoptosis in osteoblasts. J Orthop Res 1999; 17(6):  Lundskog J. Heat and bone tissue: an experimental investigation of the thermal properties of bone and threshold levels for thermal injury. Scand J Plast Reconstr Surg 1972; 9: 1-80.
8 BoneWelding Technology for Fixation of Implants to Bone The Open Orthopaedics Journal, 2009, Volume 3 47  Eriksson A, Albrektsson T, Grane B, McQueen D. Thermal injury to bone: a vital-microscopic description of heat effects. Int J Oral Surg 1982; 11(2):  Mainil-Varlet P, Rahn B, Gogolewski S. Long-term in vivo degradation and bone reaction to various polylactides. 1: One-year results. Biomaterials 1997; 18(3):  Lewandrowski KU, Lorente C, Schomacker KT, Flotte TJ, Wilkes JW, Deutsch TF. Use of the Er:YAG laser for improved plating in maxillofacial surgery: comparison of bone healing in laser and drill osteotomies. Lasers Surg Med 1996; 19(1):  Weinans H, Huiskes R, Grootenboer HJ. Quantitative analysis of bone reactions to relative motions at implant-bone interfaces. J Biomech 1993; 26(11):  Wieland M, Textor M, Chehroudi B, Brunette DM. Synergistic interaction of topographic features in the production of bone-like nodules on Ti surfaces by rat osteoblasts. Biomaterials 2005; 26(10):  Zinger O, Zhao G, Schwartz Z, et al. Differential regulation of osteoblasts by substrate microstructural features. Biomaterials 2005; 26(14):  Bergsma EJ, Rozema FR, Bos RR, de Bruijn WC. Foreign body reactions to resorbable poly(l-lactide) bone plates and screws used for the fixation of unstable zygomatic fractures. J Oral Maxillofac Surg 1993; 51(6):  Donath K, Laass M, Gunzl HJ. The histopathology of different foreign-body reactions in oral soft tissue and bone tissue. Virchows Arch A Pathol Anat Histopathol 1992; 420(2):  Hoffmann R, Weller A, Helling HJ, Krettek C, Rehm KE. Local foreign body reactions to biodegradable implants: a classification. Unfallchirurg 1997; 100(8): Received: April 2, 2009 Revised: April 27, 2009 Accepted: May 12, 2009 Langhoff et al.; Licensee Bentham Open. This is an open access article licensed under the terms of the Creative Commons Attribution Non-Commercial License (http://creativecommons.org/licenses/bync/3.0/) which permits unrestricted, non-commercial use, distribution and reproduction in any medium, provided the work is properly cited.
Journal of Materials Processing Technology 92±93 (1999) 302±308 Temperature effects in the drilling of human and bovine bone M.T. Hillery a,*, I. Shuaib b a Department of Manufacturing and Operations Engineering,
Ontario Health Technology Assessment Series 2004; Vol. 4, No. 2 Computer-Assisted Hip and Knee Arthroplasty. Navigation and Active Robotic Systems An Evidence-Based Analysis February 2004 Medical Advisory
NCB Periprosthetic Femur Plate System Surgical Technique NCB Periprosthetic Femur System Surgical Technique 3 Table of Contents Introduction 4 System Features and Benefits 9 Indications and Contraindications
Dental Traumatology 2004; 20: 203 211 Printed in Denmark. All rights reserved Copyright Ó Blackwell Munksgaard 2004 DENTAL TRAUMATOLOGY Healing of 400 intra-alveolar root fractures. 2. Effect of treatment
Chapter - E ROCK MECHANICS & GEOTECHNICAL APPLICATIONS 454 23 rd Effect of the Stress State on Waterjet Performance in Rock Slotting R. Ciccu, B. Grosso Department of Civil and Environmental Engineering
Defining and Testing EMR Usability: Principles and Proposed Methods of EMR Usability Evaluation and Rating HIMSS EHR Usability Task Force June 2009 CONTENTS EXECUTIVE SUMMARY... 1 INTRODUCTION... 2 WHAT
BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS DEPARTMENT OF STRUCTURAL MECHANICS The mechanical behavior of the bone microstructure around dental implants Summary and Theses of PhD dissertation ÉVA LAKATOS
10 Things You Need To Know About Infrared Windows See See What You ve Been Missing! Chapter List Foreword ii 1. What is an Infrared Window? 1 2. Infrared Window Lens Materials 3 3. The Importance of Emissivity
Mechanical and Microstructural Properties es of Monolithic Zirconia Crown Fracture Resistance and Impact of Low-Temperature Degradation Keisuke Nakamura Department of Prosthetic Dentistry/Dental Materials
Melting Point Determination Application Note #1 Introduction A few basic guidelines must be carefully followed to avoid errors during melting point determinations with OptiMelt. The way in which the sample
British Orthopaedic Association PATRON: H.R.H. THE PRINCE OF WALES THE CARE OF PATIENTS WITH FRAGILITY FRACTURE Published by the British Orthopaedic Association September 2007 Age Anaesthesia Association
Does Automated White-Box Test Generation Really Help Software Testers? Gordon Fraser 1 Matt Staats 2 Phil McMinn 1 Andrea Arcuri 3 Frank Padberg 4 1 Department of 2 Division of Web Science 3 Simula Research
Measuring Rev. Adv. Mater. and analyzing Sci. 29 (2011) leakage 31-53 current for outdoor insulators and specimens 31 MEASURING AND ANALYZING LEAKAGE CURRENT FOR OUTDOOR INSULATORS AND SPECIMENS Dionisios
Anders Björkman Leg. Läkare Akademisk avhandling Som med vederbörligt tillstånd av Medicinska Fakulteten vid Lunds Universitet för avläggande av doktorsexamen i medicinsk vetenskap kommer att offentligen
Pa mphl e t73 At mo s p h e r i cmo n i t o r i n g Eq u i p me n tf o rch l o r i n e Ed i t i o n7 J une2003 Table of Contents 1. INTRODUCTION... 1 1.1 PURPOSE... 1 1.2 RESPONSIBLE CARE... 1 1.3 BACKGROUND...
Università Campus Bio-Medico di Roma School of Engineering PhD Course in Biomedical Engineering (XX 2004/2007) Development and early HTA of novel microfluidic systems for bio-analytical and drug delivery
Physical Security Devices for Computer Subsystems: A Survey of Attacks and Defenses Steve H. Weingart Secure Systems and Smart Card Group IBM Thomas J. Watson Research Center Hawthorne, NY firstname.lastname@example.org
Invited Talk: Introduction to ElectromigrationAware Physical Design Jens Lienig 1st Author Dresden University 2nd Author of Technology 3rd Author 1st author's affiliation Institute of Electromechanical
HZPPOCAMPUS, VOL. 3, NO. 3, PAGES 317-3303 JULY 1993 Phase Relationship Between Hippocampal Place Units and the EEG Theta Rhythm John O'Keefe and Michael L. Recce Department of Anatomy and Developmental
Can political science literatures be believed? A study of publication bias in the APSR and the AJPS Alan Gerber Yale University Neil Malhotra Stanford University Abstract Despite great attention to the